LMucko/crystallography-open-database huggingface dataset:
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL2c
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007259
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL2c
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum
'Al0.064 Cr1.75 Fe0.002 Mg0.99 O4 V0.19 Zn0.006'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3334
_cell_length_b                   8.3334
_cell_length_c                   8.3334
_cell_formula_units_Z            8
_cell_volume                     578.718
_database_code_amcsd             0008850
_exptl_crystal_density_diffrn    4.383
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Mg.99 Fe.002 Zn.006 Al.064 V.19 Cr1.75 O4'
_cod_database_code               9007259
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL2b
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007260
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL2b
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum
'Al0.078 Cr1.67 Fe0.003 Mg0.97 Mn0.002 O4 V0.26 Zn0.005'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3369
_cell_length_b                   8.3369
_cell_length_c                   8.3369
_cell_formula_units_Z            8
_cell_volume                     579.447
_database_code_amcsd             0008851
_exptl_crystal_density_diffrn    4.364
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Mg.97 Fe.003 Mn.002 Zn.005 Al.078 V.26 Cr1.67 O4'
_cod_database_code               9007260
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1r
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007261
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1r
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum
'Al0.028 Cr1.46 Fe0.009 Mg0.99 Mn0.003 O4 V0.512 Zn0.005'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3584
_cell_length_b                   8.3584
_cell_length_c                   8.3584
_cell_formula_units_Z            8
_cell_volume                     583.942
_database_code_amcsd             0008852
_exptl_crystal_density_diffrn    4.363
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Mg.99 Fe.009 Mn.003 Zn.005 (Al.028 V.512 Cr1.46) O4'
_cod_database_code               9007261
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1p
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007262
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1p
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum
'Al0.09 Cr1.38 Fe0.018 Mg0.979 Mn0.004 O4 V0.524 Zn0.005'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3479
_cell_length_b                   8.3479
_cell_length_c                   8.3479
_cell_formula_units_Z            8
_cell_volume                     581.744
_database_code_amcsd             0008853
_exptl_crystal_density_diffrn    4.344
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Mg.979 Fe.018 Mn.004 Zn.005 Al.09 V.524 Cr1.38 O4'
_cod_database_code               9007262
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1a
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007263
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1a
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum
'Al0.086 Cr1.36 Fe0.01 Mg0.99 Mn0.003 O4 V0.55 Zn0.005'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3613
_cell_length_b                   8.3613
_cell_length_c                   8.3613
_cell_formula_units_Z            8
_cell_volume                     584.550
_database_code_amcsd             0008854
_exptl_crystal_density_diffrn    4.322
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Mg.99 Fe.01 Mn.003 Zn.005 Al.086 V.55 Cr1.36 O4'
_cod_database_code               9007263
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1b
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007264
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1b
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum
'Al0.09 Cr1.36 Fe0.01 Mg0.987 Mn0.003 O4 V0.552 Zn0.005'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3511
_cell_length_b                   8.3511
_cell_length_c                   8.3511
_cell_formula_units_Z            8
_cell_volume                     582.413
_database_code_amcsd             0008855
_exptl_crystal_density_diffrn    4.341
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Mg.987 Fe.01 Mn.003 Zn.005 Al.09 V.552 Cr1.36 O4'
_cod_database_code               9007264
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL3a
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007265
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL3a
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum
'Al0.02 Cr1.4 Fe0.005 Mg0.99 Mn0.002 O4 V0.58 Zn0.008'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3664
_cell_length_b                   8.3664
_cell_length_c                   8.3664
_cell_formula_units_Z            8
_cell_volume                     585.620
_database_code_amcsd             0008856
_exptl_crystal_density_diffrn    4.352
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum
'Mg.99 Fe.005 Mn.002 Zn.008 (Al.02 V.58 Cr1.4) O4'
_cod_database_code               9007265
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1d
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007266
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1d
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum
'Al0.024 Cr1.36 Fe0.004 Mg0.99 Mn0.003 O4 V0.64'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3604
_cell_length_b                   8.3604
_cell_length_c                   8.3604
_cell_formula_units_Z            8
_cell_volume                     584.361
_database_code_amcsd             0008857
_exptl_crystal_density_diffrn    4.374
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Mg.99 Fe.004 Mn.003 Al.024 (V.64 Cr1.36) O4'
_cod_database_code               9007266
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1e
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007267
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL1e
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum            'Al0.02 Cr1.3 Fe0.01 Mg0.99 Mn0.003 O4 V0.68'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3629
_cell_length_b                   8.3629
_cell_length_c                   8.3629
_cell_formula_units_Z            8
_cell_volume                     584.885
_database_code_amcsd             0008858
_exptl_crystal_density_diffrn    4.351
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Mg.99 Fe.01 Mn.003 (Al.02 V.68 Cr1.3) O4'
_cod_database_code               9007267
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL3b
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007268
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL3b
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum
'Al0.024 Cr1.24 Fe0.009 Mg0.99 O4 V0.74 Zn0.008'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3686
_cell_length_b                   8.3686
_cell_length_c                   8.3686
_cell_formula_units_Z            8
_cell_volume                     586.082
_database_code_amcsd             0008859
_exptl_crystal_density_diffrn    4.350
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Mg.99 Fe.009 Zn.008 Al.024 V.74 Cr1.24 O4'
_cod_database_code               9007268
Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake Baikal, Russia): the influence of V3+ on structural stability Sample: VRL3c
Lavina, B.; Reznitskii, L. Z.; Bosi, F.; Physics and Chemistry of Minerals 30 (2003) 599–605; doi:10.1007/s00269-003-0354-y

data_9007269
_publ_section_title
;Crystal chemistry of some Mg, Cr, V normal spinels from Sludyanka (Lake
 Baikal, Russia): the influence of V3+ on structural stability Sample: VRL3c
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              599
_journal_page_last               605
_journal_paper_doi               10.1007/s00269-003-0354-y
_journal_volume                  30
_journal_year                    2003
_chemical_compound_source        'Sludyanka, Lake Baikal, Russia'
_chemical_formula_sum            'Al0.02 Cr1.02 Fe0.002 Mg O4 V0.96 Zn0.015'
_chemical_name_mineral           Magnesiochromite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3800
_cell_length_b                   8.3800
_cell_length_c                   8.3800
_cell_formula_units_Z            8
_cell_volume                     588.480
_database_code_amcsd             0008860
_exptl_crystal_density_diffrn    4.331
_cod_original_cell_volume        588.481
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Mg Fe.002 Zn.015 (Al.02 V.96 Cr1.02) O4'
_cod_database_code               9007269
Single-crystal X-ray diffraction study of cation distribution in MgAl2O4-MgFe2O4 spinel solid solution Sample: T = 23 C, x = 1.21
Nakatsuka, A.; Ueno, H.; Nakayama, N.; Mizota, T.; Maekawa, H.; Physics and Chemistry of Minerals 31 (2004) 278–287; doi:10.1007/s00269-004-0385-z

data_9007270
_publ_section_title
;
 Single-crystal X-ray diffraction study of cation distribution
 in MgAl2O4-MgFe2O4 spinel solid solution
 Sample: T = 23 C, x = 1.21
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              278
_journal_page_last               287
_journal_paper_doi               10.1007/s00269-004-0385-z
_journal_volume                  31
_journal_year                    2004
_chemical_formula_sum            'Al0.79 Fe1.21 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.2796
_cell_length_b                   8.2796
_cell_length_c                   8.2796
_cell_formula_units_Z            8
_cell_volume                     567.581
_database_code_amcsd             0008861
_diffrn_ambient_temperature      296.15
_exptl_crystal_density_diffrn    4.147
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Al.79 Fe1.21) O4'
_cod_database_code               9007270
Single-crystal X-ray diffraction study of cation distribution in MgAl2O4-MgFe2O4 spinel solid solution Sample: T = 23 C, x = 1.53
Nakatsuka, A.; Ueno, H.; Nakayama, N.; Mizota, T.; Maekawa, H.; Physics and Chemistry of Minerals 31 (2004) 278–287; doi:10.1007/s00269-004-0385-z

data_9007271
_publ_section_title
;
 Single-crystal X-ray diffraction study of cation distribution
 in MgAl2O4-MgFe2O4 spinel solid solution
 Sample: T = 23 C, x = 1.53
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              278
_journal_page_last               287
_journal_paper_doi               10.1007/s00269-004-0385-z
_journal_volume                  31
_journal_year                    2004
_chemical_formula_sum            'Al0.47 Fe1.52 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3252
_cell_length_b                   8.3252
_cell_length_c                   8.3252
_cell_formula_units_Z            8
_cell_volume                     577.011
_database_code_amcsd             0008862
_diffrn_ambient_temperature      296.15
_exptl_crystal_density_diffrn    4.279
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Mg Al.47 Fe1.52 O4'
_cod_database_code               9007271
Single-crystal X-ray diffraction study of cation distribution in MgAl2O4-MgFe2O4 spinel solid solution Sample: T = 23 C, x = 1.77
Nakatsuka, A.; Ueno, H.; Nakayama, N.; Mizota, T.; Maekawa, H.; Physics and Chemistry of Minerals 31 (2004) 278–287; doi:10.1007/s00269-004-0385-z

data_9007272
_publ_section_title
;
 Single-crystal X-ray diffraction study of cation distribution
 in MgAl2O4-MgFe2O4 spinel solid solution
 Sample: T = 23 C, x = 1.77
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              278
_journal_page_last               287
_journal_paper_doi               10.1007/s00269-004-0385-z
_journal_volume                  31
_journal_year                    2004
_chemical_formula_sum            'Al0.22 Fe1.77 Mg1.01 O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3422
_cell_length_b                   8.3422
_cell_length_c                   8.3422
_cell_formula_units_Z            8
_cell_volume                     580.553
_database_code_amcsd             0008863
_diffrn_ambient_temperature      296.15
_exptl_crystal_density_diffrn    4.424
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Mg1.01 Fe1.77 Al.22 O4'
_cod_database_code               9007272
Single-crystal X-ray diffraction study of cation distribution in MgAl2O4-MgFe2O4 spinel solid solution Sample: T = 23 C, x = 2.00
Nakatsuka, A.; Ueno, H.; Nakayama, N.; Mizota, T.; Maekawa, H.; Physics and Chemistry of Minerals 31 (2004) 278–287; doi:10.1007/s00269-004-0385-z

data_9007273
_publ_section_title
;
 Single-crystal X-ray diffraction study of cation distribution
 in MgAl2O4-MgFe2O4 spinel solid solution
 Sample: T = 23 C, x = 2.00
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              278
_journal_page_last               287
_journal_paper_doi               10.1007/s00269-004-0385-z
_journal_volume                  31
_journal_year                    2004
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3600
_cell_length_b                   8.3600
_cell_length_c                   8.3600
_cell_formula_units_Z            8
_cell_volume                     584.277
_database_code_amcsd             0008864
_diffrn_ambient_temperature      296.15
_exptl_crystal_density_diffrn    4.547
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9007273